Synthesis, Structure, and Magnetic Properties of A2Cu5(TeO3)(SO4)3(OH)4 (A = Na, K): The First Compounds with a 1D Kagomé Strip Lattice.
Tang, Yingying; Guo, Wenbin; Xiang, Hongping; Zhang, Suyun; Yang, Ming; Cui, Meiyan; Wang, Nannan; He, Zhangzhen; Inorganic chemistry 55 (2016) 644–648; doi:10.1021/acs.inorgchem.5b01889

data_4344583
_publ_section_title
;
 Synthesis, Structure, and Magnetic Properties of A2Cu5(TeO3)(SO4)3(OH)4
 (A = Na, K): The First Compounds with a 1D Kagom\'e Strip Lattice.
;
_journal_issue                   2
_journal_name_full               'Inorganic chemistry'
_journal_page_first              644
_journal_page_last               648
_journal_paper_doi               10.1021/acs.inorgchem.5b01889
_journal_volume                  55
_journal_year                    2016
_chemical_formula_moiety         'Cu5 Na2 O19 S3 Te'
_chemical_formula_sum            'Cu5 Na2 O19 S3 Te'
_chemical_formula_weight         891.51
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           11
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 111.160(6)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   7.294(3)
_cell_length_b                   12.005(4)
_cell_length_c                   9.214(3)
_cell_measurement_reflns_used    2293
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4895
_cell_measurement_theta_min      2.3704
_cell_volume                     752.4(5)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 14.6306
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0218
_diffrn_reflns_av_sigmaI/netI    0.0222
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            5846
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         2.37
_exptl_absorpt_coefficient_mu    9.438
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.660
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    3.935
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Prism
_exptl_crystal_F_000             838
_exptl_crystal_size_max          0.2000
_exptl_crystal_size_mid          0.2000
_exptl_crystal_size_min          0.2000
_refine_diff_density_max         0.686
_refine_diff_density_min         -1.110
_refine_diff_density_rms         0.217
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.093
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     151
_refine_ls_number_reflns         1806
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.093
_refine_ls_R_factor_all          0.0221
_refine_ls_R_factor_gt           0.0204
_refine_ls_shift/su_max          0.083
_refine_ls_shift/su_mean         0.013
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0340P)^2^+0.3852P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0545
_refine_ls_wR_factor_ref         0.0555
_reflns_number_gt                1699
_reflns_number_total             1812
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic5b01889_si_003.cif
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/usr/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 
;
_cod_original_sg_symbol_H-M      P21/M
_cod_database_code               4344583